TSpace Research Repository tspace.library.utoronto.ca
Efficient tandem solar cells with solution-
processed perovskite on textured crystalline
Yi Hou, Erkan Aydin, Michele De Bastiani, Chuanxiao Xiao,
Furkan H. Isikgor, Ding-Jiang Xue, Bin Chen, Hao Chen, Behzad
Bahrami, Ashraful H. Chowdhury, Andrew Johnston, Se-Woong
Baek, Ziru Huang, Mingyang Wei, Yitong Dong, Joel Troughton,
Rawan Jalmood, Alessandro J. Mirabelli, Thomas G. Allen,
Emmanuel Van Kerschaver, Makhsud I. Saidaminov, Derya Baran,
Qiquan Qiao, Kai Zhu, Stefaan De Wolf, Edward H. Sargent
Hou, Y., Aydin, E., De Bastiani, M., Xiao, C., Isikgor, F. H., Xue, D.-J.,
Chen, B., Chen, H., Bahrami, B., Chowdhury, A. H., Johnston, A.,
Baek, S.-W., Huang, Z., Wei, M., Dong, Y., Troughton, J., Jalmood, R.,
Mirabelli, A. J., Allen, T. G., Sargent, E. H. (2020). Efficient tandem
solar cells with solution-processed perovskite on textured crystalline
silicon. Science, 367(6482), 1135.
Publisher’s Statement This is the author’s version of the work. It is posted here by
permission of the AAAS for personal use, not for redistribution.
The definitive version was published in Science Volume 367 on
April 6, 2020, DOI: 10.1126/science.aaz3691.
How to cite TSpace items
Always cite the published version, so the author(s) will receive recognition through services that track
citation counts, e.g. Scopus. If you need to cite the page number of the author manuscript from TSpace
because you cannot access the published version, then cite the TSpace version in addition to the published
version using the permanent URI (handle) found on the record page.
This article was made openly accessible by U of T Faculty.
Please tell us how this access benefits you. Your story matters.
Efficient tandem solar cells with solution-processed perovskite on
textured crystalline silicon
Yi Hou,1† Erkan Aydin,2† Michele De Bastiani,2† Chuanxiao Xiao,3† Furkan H. Isikgor,2 Ding-
Jiang Xue,1 Bin Chen,1 Hao Chen,1 Behzad Bahrami,4 Ashraful H. Chowdhury,4 Andrew
Johnston1, Se-Woong Baek,1 Ziru Huang,1 Mingyang Wei,1 Yitong Dong,1 Joel Troughton,2
Rawan Jalmood,2 Alessandro J. Mirabelli,2 Thomas Allen,2 Emmanuel Van Kerschaver,2 Makhsud
I. Saidaminov,1 Derya Baran,2 Qiquan Qiao,4 Kai Zhu,3 Stefaan De Wolf,2* and Edward H.
1Department of Electrical and Computer Engineering, University of Toronto, Toronto, Ontario
M5S 1A4, Canada
2KAUST Solar Center (KSC), Physical Sciences and Engineering Division (PSE), King Abdullah
University of Science and Technology (KAUST), Thuwal 23955-6900, Kingdom of Saudi Arabia
3National Renewable Energy Laboratory (NREL), Golden, Colorado 80401, USA
4Department of Electrical Engineering, Center for Advanced Photovoltaics, South Dakota State
University, Brookings, South Dakota 57007, USA
†These authors contributed equally to this work.
*Correspondence to: E-mail: email@example.com (S.D.W.); firstname.lastname@example.org
Abstract: Stacking solar cells with decreasing band gaps to form tandems offers to overcome the
single-junction Shockley-Queisser limit in photovoltaics. The rapid development of solution-
processed perovskites has brought perovskite single-junction efficiencies > 20%. However, this
process has yet to enable monolithic integration with industry-relevant textured crystalline silicon
solar cells. We report tandems that combine solution-processed micrometer-thick perovskite top
cells with fully-textured silicon heterojunction bottom cells. To overcome the charge-collection
challenges in micrometer-thick perovskites, we enhance threefold the depletion width at the bases
of silicon pyramids. Moreover, by anchoring a self-limiting passivant (1-butanethiol) on the
perovskite surfaces, we enhanced the diffusion length and further suppressed phase segregation.
These combined enhancements enabled independently certified power conversion efficiency of
25.7% for perovskite/silicon tandem solar cells. These devices exhibited negligible performance
loss after a 400-hour thermal stability test at 85 Celsius and also after 400 hours under maximum
power point tracking at 40 Celsius.
Through an intensive worldwide effort, perovskite solar cell (PSC) power conversion efficiencies
(PCEs) have increased from an initial 3.8% to a remarkable certified 25.2% during the last decade
(1, 2). This progress is based on the combination of remarkable materials properties such as a low
energy required for crystal formation (3), a sharp optical absorption edge (4), and a tunable
bandgap (5) ideally suited for photovoltaic (PV) applications. The rapid development of PSCs is
further enabled by the use of solution-based coating methods to deposit the semiconductors (6).
These properties also make PSCs attractive as top cells for tandem applications that use lower band
gap bottom cells such as crystalline silicon (c-Si) and CIGS (7-18). By reducing thermalization
losses, stacking PV absorbers of decreasing band gap in a multijunction device can overcome the
Shockley-Queisser efficiency limit of 33.7% for single-junction solar cells. The combination with
a c-Si bottom cell is of particular appeal, as single-junction c-Si based technology has come to
dominate the PV market. However, as c-Si solar cell efficiencies approach their practical limits,
multijunction technologies using a c-Si bottom cell are of interest to drive further efficiency
Silicon heterojunction (SHJ) technology is attractive for tandem solar cells because of its high PCE
and comparatively straightforward tandem integration. At present, most reported monolithic
perovskite/silicon tandem devices are based on a single-side texturing configuration: c-Si wafers
with their front flat-polished so that it is compatible with existing solution-based perovskite
fabrication processes, and a textured back side for enhanced light trapping relative to the case of a
double-side polished c-Si device (8, 14-16, 18). This configuration, however, provides limited
light-trapping benefits, and requires additional antireflection foils that do not provide sufficient
light trapping compared to the textured counterpart (18). Further, the effectiveness of antireflection
foils can be compromised upon encapsulation, and surface-polishing methods increase
As a result, recent attention has shifted to combining perovskite with fully textured c-Si (7). The
benefits of fully-textured tandems have been demonstrated previously by Sahli et al. using a hybrid
two-step deposition method combining sequential co-evaporation of PbI2 and CsBr and solution
conversion (7). Unfortunately, the fill factor (FF) was moderate, a result of limited perovskite
quality achieved using this approach (19, 20). More efficient—but also more complex—thermal
co-evaporation enables textured tandems; however, the large vapor-pressure difference between
the organic and inorganic components demands a high level of control over the deposition rates of
each precursor during the evaporation process (21).
Early efforts to deposit perovskites by using solution techniques on top of micrometer-sized Si
pyramids quickly revealed a number of hurdles: uncovered Si pyramids, shunt paths, and
inefficient charge collection in films with variable thickness. In addition, the application of
conventional surface-passivation techniques—a prerequisite for state-of-art PSC device
performance—are incompatible with the rough perovskite surfaces that result from the underlying
c-Si texture (7). So far, insulating solution-processed passivants have failed to cover rough surfaces
with the needed consistency of thickness of a few nanometers.
Previous reports of perovskite-silicon tandems atop textured c-Si bottom cells have relied on
physical vapor deposition of the perovskite front cell, rather than solution-processed perovskite
cells on textured c-Si bottom cells. We sought to develop a high-quality micrometer-thick
perovskite to cover the pyramids; and, simultaneously, to enhance charge collection in these thick
films through improved drift and diffusion of photo-generated carriers. We combined solution-
processed, micrometer-thick, wide-band gap perovskite solar cells with pyramidal-textured c-Si
bottom cells. This approach achieved a threefold enhanced depletion width in the perovskite
semiconductor at the valleys of Si pyramids, improving carrier collection, as revealed using
nanometer-scale Kelvin probe force microscopy (KPFM).
To further increase carrier diffusion length, we introduce a conformal surface-passivation strategy
for rough surfaces by anchoring a self-limiting passivant on the wide-bandgap perovskite surface.
This passivant also suppresses phase segregation. In addition, micrometer-thick perovskites allow